#------------------------------------------------------------------------------
#$Date: 2016-03-26 17:36:08 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180400 $
#$URL: svn://www.crystallography.net/cod/cif/7/20/69/7206931.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7206931
loop_
_publ_author_name
'Lv, Yao-Kang'
'Jiang, Zhan-Guo'
'Gan, Li-Hua'
'Liu, Ming-Xian'
'Feng, Yun-Long'
_publ_section_title
;
 Three novel organic-inorganic hybrid materials based on decaoxovanadates
 obtained from a new liquid phase reaction
;
_journal_issue                   1
_journal_name_full               CrystEngComm
_journal_page_first              314
_journal_paper_doi               10.1039/c1ce05605k
_journal_volume                  14
_journal_year                    2012
_chemical_formula_moiety         'H4 O28 V10, 2(C7 H15 N4 O), 6(H2 O)'
_chemical_formula_sum            'C14 H46 N8 O36 V10'
_chemical_formula_weight         1411.99
_chemical_name_systematic
;
?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                103.250(2)
_cell_angle_beta                 98.612(2)
_cell_angle_gamma                102.932(2)
_cell_formula_units_Z            1
_cell_length_a                   9.4462(4)
_cell_length_b                   10.6899(4)
_cell_length_c                   10.9170(4)
_cell_measurement_reflns_used    6194
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.52
_cell_measurement_theta_min      1.96
_cell_volume                     1022.07(7)
_computing_cell_refinement       'SAINT (Bruker, 2006)'
_computing_data_collection       'APEXII (Bruker, 2006)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXTL (Bruker, 2002)'
_computing_publication_material  SHELXTL
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker APEX-II area-detector diffractometer'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0268
_diffrn_reflns_av_sigmaI/netI    0.0272
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            17412
_diffrn_reflns_theta_full        27.52
_diffrn_reflns_theta_max         27.52
_diffrn_reflns_theta_min         1.96
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    2.301
_exptl_absorpt_correction_T_max  0.86
_exptl_absorpt_correction_T_min  0.66
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'SADABS (Sheldrick, 1996)'
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    2.294
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       sheet
_exptl_crystal_F_000             704
_exptl_crystal_size_max          0.293
_exptl_crystal_size_mid          0.157
_exptl_crystal_size_min          0.065
_refine_diff_density_max         0.699
_refine_diff_density_min         -0.760
_refine_diff_density_rms         0.082
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.011
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     334
_refine_ls_number_reflns         4686
_refine_ls_number_restraints     13
_refine_ls_restrained_S_all      1.013
_refine_ls_R_factor_all          0.0387
_refine_ls_R_factor_gt           0.0295
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0451P)²+0.8534P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0792
_refine_ls_wR_factor_ref         0.0859
_reflns_number_gt                3889
_reflns_number_total             4686
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            c1ce05605k.txt
_cod_data_source_block           a
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               7206931
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
V1 V 0.38635(5) 0.56383(4) 0.27970(4) 0.01809(11) Uani 1 1 d .
V2 V 0.63061(4) 0.46664(4) 0.42722(4) 0.01583(10) Uani 1 1 d .
V3 V 0.38694(5) 0.26473(4) 0.20806(4) 0.02026(11) Uani 1 1 d .
V4 V 0.14045(5) 0.34995(4) 0.33225(4) 0.02102(11) Uani 1 1 d .
V5 V 0.36907(5) 0.23516(4) 0.47996(4) 0.01835(11) Uani 1 1 d D
O1 O 0.39894(19) 0.16112(16) 0.31945(16) 0.0216(4) Uani 1 1 d .
O1W O 0.7653(2) 0.1776(2) 0.4381(2) 0.0339(5) Uani 1 1 d D
H1WA H 0.811(3) 0.155(3) 0.493(2) 0.041 Uiso 1 1 d D
H1WB H 0.829(3) 0.224(3) 0.411(3) 0.041 Uiso 1 1 d D
O2 O 0.59991(18) 0.61144(15) 0.36574(15) 0.0169(3) Uani 1 1 d .
O2W O 0.6986(3) 0.1363(3) 0.0255(3) 0.0662(8) Uani 1 1 d D
H2WA H 0.703(4) 0.217(2) 0.037(4) 0.079 Uiso 1 1 d D
H2WB H 0.782(3) 0.133(4) 0.012(4) 0.079 Uiso 1 1 d D
O3 O 0.60841(18) 0.35208(16) 0.28614(16) 0.0199(4) Uani 1 1 d .
O3W O 0.4497(4) 0.0221(4) 0.7983(3) 0.0773(9) Uani 1 1 d D
H3WA H 0.385(4) -0.022(4) 0.831(4) 0.093 Uiso 1 1 d D
H3WB H 0.520(4) 0.063(4) 0.869(3) 0.093 Uiso 1 1 d D
O4 O 0.40265(18) 0.67163(16) 0.47124(15) 0.0171(3) Uani 1 1 d D
H4 H 0.342(3) 0.721(2) 0.486(3) 0.021 Uiso 1 1 d D
O5 O 0.18855(19) 0.24458(17) 0.19646(16) 0.0227(4) Uani 1 1 d .
O6 O 0.18754(18) 0.49772(17) 0.27495(16) 0.0221(4) Uani 1 1 d .
O7 O 0.40063(19) 0.42970(17) 0.15929(16) 0.0214(4) Uani 1 1 d .
O8 O 0.39982(17) 0.41807(15) 0.40170(15) 0.0167(3) Uani 1 1 d .
O9 O 0.81395(18) 0.52175(17) 0.48773(16) 0.0208(4) Uani 1 1 d .
O10 O 0.18068(19) 0.22851(16) 0.43201(16) 0.0219(4) Uani 1 1 d .
O11 O 0.3892(2) 0.68289(18) 0.21235(17) 0.0281(4) Uani 1 1 d .
O12 O 0.3684(2) 0.11954(18) 0.55084(19) 0.0282(4) Uani 1 1 d D
H12 H 0.419(3) 0.067(2) 0.537(3) 0.034 Uiso 1 1 d D
O13 O 0.3986(2) 0.16832(18) 0.07649(17) 0.0295(4) Uani 1 1 d .
O14 O -0.0378(2) 0.3105(2) 0.30093(19) 0.0316(4) Uani 1 1 d .
O15 O 0.1517(3) 0.5675(2) 0.8861(2) 0.0471(6) Uani 1 1 d D
H15 H 0.141(4) 0.580(4) 0.808(2) 0.057 Uiso 1 1 d D
N1 N -0.0425(2) 0.1628(2) 0.6637(2) 0.0259(5) Uani 1 1 d .
N2 N 0.1525(2) 0.1048(2) 0.7921(2) 0.0241(5) Uani 1 1 d .
N3 N -0.0481(3) 0.1659(2) 0.8859(2) 0.0292(5) Uani 1 1 d .
N4 N 0.1373(2) 0.3340(2) 0.8371(2) 0.0221(4) Uani 1 1 d .
C1 C 0.0598(3) 0.0769(3) 0.6633(2) 0.0260(6) Uani 1 1 d .
H1A H 0.0028 -0.0160 0.6353 0.031 Uiso 1 1 calc R
H1B H 0.1229 0.0919 0.6029 0.031 Uiso 1 1 calc R
C2 C 0.2394(3) 0.2419(2) 0.8332(2) 0.0232(5) Uani 1 1 d .
H2A H 0.3041 0.2581 0.7742 0.028 Uiso 1 1 calc R
H2B H 0.3011 0.2602 0.9181 0.028 Uiso 1 1 calc R
C3 C 0.2363(3) 0.4773(3) 0.8834(3) 0.0342(6) Uani 1 1 d .
H3A H 0.2949 0.4925 0.9689 0.041 Uiso 1 1 calc R
H3B H 0.3041 0.4907 0.8262 0.041 Uiso 1 1 calc R
C4 C 0.0552(3) 0.0805(3) 0.8824(3) 0.0285(6) Uani 1 1 d .
H4A H 0.1154 0.0989 0.9679 0.034 Uiso 1 1 calc R
H4B H -0.0012 -0.0125 0.8561 0.034 Uiso 1 1 calc R
C5 C -0.1385(3) 0.1374(3) 0.7549(3) 0.0325(6) Uani 1 1 d .
H5A H -0.1968 0.0450 0.7269 0.039 Uiso 1 1 calc R
H5B H -0.2065 0.1933 0.7561 0.039 Uiso 1 1 calc R
C6 C 0.0416(3) 0.3010(3) 0.7026(2) 0.0259(6) Uani 1 1 d .
H6A H -0.0257 0.3576 0.7024 0.031 Uiso 1 1 calc R
H6B H 0.1043 0.3176 0.6422 0.031 Uiso 1 1 calc R
C7 C 0.0358(3) 0.3045(3) 0.9290(3) 0.0277(6) Uani 1 1 d .
H7A H 0.0949 0.3236 1.0152 0.033 Uiso 1 1 calc R
H7B H -0.0317 0.3610 0.9318 0.033 Uiso 1 1 calc R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O11 V1 O7 104.85(9) . .
O11 V1 O6 103.36(9) . .
O7 V1 O6 96.25(8) . .
O11 V1 O2 99.64(8) . .
O7 V1 O2 93.61(7) . .
O6 V1 O2 151.65(7) . .
O11 V1 O4 98.92(8) . .
O7 V1 O4 154.69(7) . .
O6 V1 O4 86.48(7) . .
O2 V1 O4 73.70(7) . .
O11 V1 O8 171.79(8) . .
O7 V1 O8 82.03(7) . .
O6 V1 O8 79.98(7) . .
O2 V1 O8 75.16(6) . .
O4 V1 O8 73.65(6) . .
O11 V1 V4 135.24(7) . .
O7 V1 V4 84.02(6) . .
O6 V1 V4 32.04(5) . .
O2 V1 V4 123.88(5) . .
O4 V1 V4 85.22(5) . .
O8 V1 V4 48.91(4) . .
O11 V1 V3 139.13(7) . .
O7 V1 V3 34.39(5) . .
O6 V1 V3 84.37(5) . .
O2 V1 V3 89.01(5) . .
O4 V1 V3 121.76(4) . .
O8 V1 V3 48.11(4) . .
V4 V1 V3 59.246(13) . .
O11 V1 V2 134.20(7) . .
O7 V1 V2 78.47(6) . .
O6 V1 V2 121.91(5) . .
O2 V1 V2 35.27(4) . .
O4 V1 V2 78.78(5) . .
O8 V1 V2 41.94(4) . .
V4 V1 V2 90.458(15) . .
V3 V1 V2 59.077(13) . .
O9 V2 O3 106.17(8) . .
O9 V2 O2 99.79(8) . .
O3 V2 O2 99.75(8) . .
O9 V2 O4 94.20(8) . 2_666
O3 V2 O4 93.92(7) . 2_666
O2 V2 O4 156.81(7) . 2_666
O9 V2 O8 165.03(7) . .
O3 V2 O8 87.92(7) . .
O2 V2 O8 82.32(7) . .
O4 V2 O8 79.54(6) 2_666 .
O9 V2 O8 87.91(7) . 2_666
O3 V2 O8 164.91(7) . 2_666
O2 V2 O8 82.75(6) . 2_666
O4 V2 O8 79.36(6) 2_666 2_666
O8 V2 O8 77.62(7) . 2_666
O9 V2 V3 144.71(6) . .
O3 V2 V3 38.73(6) . .
O2 V2 V3 92.27(5) . .
O4 V2 V3 86.75(5) 2_666 .
O8 V2 V3 49.20(4) . .
O8 V2 V3 126.69(5) 2_666 .
O9 V2 V4 38.27(6) . 2_666
O3 V2 V4 144.21(6) . 2_666
O2 V2 V4 92.72(5) . 2_666
O4 V2 V4 86.87(5) 2_666 2_666
O8 V2 V4 127.15(5) . 2_666
O8 V2 V4 49.64(5) 2_666 2_666
V3 V2 V4 173.238(17) . 2_666
O9 V2 V5 85.23(6) . 2_666
O3 V2 V5 137.54(6) . 2_666
O2 V2 V5 37.84(5) . 2_666
O4 V2 V5 126.56(5) 2_666 2_666
O8 V2 V5 87.65(4) . 2_666
O8 V2 V5 47.20(4) 2_666 2_666
V3 V2 V5 121.979(16) . 2_666
V4 V2 V5 60.823(13) 2_666 2_666
O9 V2 V1 137.33(6) . .
O3 V2 V1 85.19(6) . .
O2 V2 V1 37.61(5) . .
O4 V2 V1 126.56(5) 2_666 .
O8 V2 V1 47.03(4) . .
O8 V2 V1 88.02(4) 2_666 .
V3 V2 V1 60.395(13) . .
V4 V2 V1 122.446(16) 2_666 .
V5 V2 V1 61.702(13) 2_666 .
O13 V3 O5 104.57(9) . .
O13 V3 O1 102.07(9) . .
O5 V3 O1 93.71(8) . .
O13 V3 O7 100.42(8) . .
O5 V3 O7 88.88(8) . .
O1 V3 O7 155.91(8) . .
O13 V3 O3 99.69(9) . .
O5 V3 O3 155.33(7) . .
O1 V3 O3 85.49(7) . .
O7 V3 O3 82.33(7) . .
O13 V3 O8 173.09(8) . .
O5 V3 O8 81.96(7) . .
O1 V3 O8 79.46(6) . .
O7 V3 O8 77.20(6) . .
O3 V3 O8 73.64(6) . .
O13 V3 V4 137.29(7) . .
O5 V3 V4 32.77(5) . .
O1 V3 V4 87.28(5) . .
O7 V3 V4 82.01(5) . .
O3 V3 V4 122.72(5) . .
O8 V3 V4 49.20(4) . .
O13 V3 V2 130.61(7) . .
O5 V3 V2 124.54(6) . .
O1 V3 V2 81.39(6) . .
O7 V3 V2 77.47(5) . .
O3 V3 V2 30.95(5) . .
O8 V3 V2 42.69(4) . .
V4 V3 V2 91.805(15) . .
O13 V3 V5 134.86(7) . .
O5 V3 V5 81.43(6) . .
O1 V3 V5 33.04(5) . .
O7 V3 V5 124.61(5) . .
O3 V3 V5 84.70(5) . .
O8 V3 V5 47.51(4) . .
V4 V3 V5 61.261(13) . .
V2 V3 V5 64.890(13) . .
O13 V3 V1 131.14(7) . .
O5 V3 V1 80.71(6) . .
O1 V3 V1 126.34(5) . .
O7 V3 V1 30.74(5) . .
O3 V3 V1 80.00(5) . .
O8 V3 V1 46.88(4) . .
V4 V3 V1 60.056(13) . .
V2 V3 V1 60.528(13) . .
V5 V3 V1 93.967(15) . .
O14 V4 O6 102.57(9) . .
O14 V4 O5 104.78(9) . .
O6 V4 O5 93.14(8) . .
O14 V4 O10 101.52(9) . .
O6 V4 O10 154.60(8) . .
O5 V4 O10 88.41(8) . .
O14 V4 O9 100.59(9) . 2_666
O6 V4 O9 86.38(7) . 2_666
O5 V4 O9 154.09(7) . 2_666
O10 V4 O9 81.40(7) . 2_666
O14 V4 O8 173.64(8) . .
O6 V4 O8 78.69(6) . .
O5 V4 O8 81.30(7) . .
O10 V4 O8 76.49(6) . .
O9 V4 O8 73.19(6) 2_666 .
O14 V4 V3 137.37(7) . .
O6 V4 V3 86.09(5) . .
O5 V4 V3 32.61(5) . .
O10 V4 V3 81.63(5) . .
O9 V4 V3 121.74(5) 2_666 .
O8 V4 V3 48.69(4) . .
O14 V4 V2 131.08(7) . 2_666
O6 V4 V2 81.62(6) . 2_666
O5 V4 V2 123.82(6) . 2_666
O10 V4 V2 76.54(5) . 2_666
O9 V4 V2 30.51(5) 2_666 2_666
O8 V4 V2 42.68(4) . 2_666
V3 V4 V2 91.279(15) . 2_666
O14 V4 V1 134.82(7) . .
O6 V4 V1 32.48(5) . .
O5 V4 V1 81.18(6) . .
O10 V4 V1 123.56(5) . .
O9 V4 V1 84.74(5) 2_666 .
O8 V4 V1 47.16(4) . .
V3 V4 V1 60.698(13) . .
V2 V4 V1 64.958(13) 2_666 .
O12 V5 O10 104.98(9) . .
O12 V5 O1 103.60(9) . .
O10 V5 O1 97.23(8) . .
O12 V5 O2 98.78(8) . 2_666
O10 V5 O2 92.71(7) . 2_666
O1 V5 O2 152.16(7) . 2_666
O12 V5 O2 98.78(8) . 2_666
O10 V5 O2 92.71(7) . 2_666
O1 V5 O2 152.16(7) . 2_666
O2 V5 O2 0.00(10) 2_666 2_666
O12 V5 O4 98.77(9) . 2_666
O10 V5 O4 154.34(7) . 2_666
O1 V5 O4 86.34(7) . 2_666
O2 V5 O4 73.95(7) 2_666 2_666
O2 V5 O4 73.95(7) 2_666 2_666
O12 V5 O8 171.64(9) . .
O10 V5 O8 81.55(7) . .
O1 V5 O8 80.39(6) . .
O2 V5 O8 75.43(6) 2_666 .
O2 V5 O8 75.43(6) 2_666 .
O4 V5 O8 73.97(6) 2_666 .
O12 V5 V3 136.21(7) . .
O10 V5 V3 83.95(6) . .
O1 V5 V3 32.82(5) . .
O2 V5 V3 123.94(5) 2_666 .
O2 V5 V3 123.94(5) 2_666 .
O4 V5 V3 85.63(5) 2_666 .
O8 V5 V3 48.66(4) . .
O12 V5 V2 133.43(7) . 2_666
O10 V5 V2 77.60(6) . 2_666
O1 V5 V2 122.45(5) . 2_666
O2 V5 V2 35.39(4) 2_666 2_666
O2 V5 V2 35.39(4) 2_666 2_666
O4 V5 V2 79.07(5) 2_666 2_666
O8 V5 V2 42.05(4) . 2_666
V3 V5 V2 90.295(14) . 2_666
V3 O1 V5 114.14(9) . .
H1WA O1W H1WB 105(2) . .
V2 O2 V1 107.13(8) . .
V2 O2 V5 106.77(8) . 2_666
V1 O2 V5 106.59(7) . 2_666
H2WA O2W H2WB 103(3) . .
V2 O3 V3 110.32(8) . .
H3WA O3W H3WB 99(2) . .
V2 O4 V5 106.08(7) 2_666 2_666
V2 O4 V1 106.02(7) 2_666 .
V5 O4 V1 99.11(7) 2_666 .
V2 O4 H4 108.0(18) 2_666 .
V5 O4 H4 118.2(18) 2_666 .
V1 O4 H4 118.2(18) . .
V3 O5 V4 114.62(9) . .
V4 O6 V1 115.48(9) . .
V1 O7 V3 114.87(9) . .
V2 O8 V2 102.38(7) . 2_666
V2 O8 V1 91.03(6) . .
V2 O8 V1 98.55(6) 2_666 .
V2 O8 V5 98.04(6) . .
V2 O8 V5 90.75(6) 2_666 .
V1 O8 V5 165.35(8) . .
V2 O8 V3 88.11(6) . .
V2 O8 V3 168.80(8) 2_666 .
V1 O8 V3 85.00(5) . .
V5 O8 V3 83.83(5) . .
V2 O8 V4 169.34(8) . .
V2 O8 V4 87.68(6) 2_666 .
V1 O8 V4 83.93(5) . .
V5 O8 V4 85.17(5) . .
V3 O8 V4 82.11(5) . .
V2 O9 V4 111.21(8) . 2_666
V5 O10 V4 115.78(9) . .
V5 O12 H12 122.7(18) . .
C3 O15 H15 105(2) . .
C6 N1 C5 109.9(2) . .
C6 N1 C1 109.7(2) . .
C5 N1 C1 108.6(2) . .
C2 N2 C1 109.7(2) . .
C2 N2 C4 109.5(2) . .
C1 N2 C4 108.8(2) . .
C7 N3 C4 109.5(2) . .
C7 N3 C5 109.6(2) . .
C4 N3 C5 108.9(2) . .
C2 N4 C6 107.92(19) . .
C2 N4 C7 108.26(19) . .
C6 N4 C7 108.5(2) . .
C2 N4 C3 107.3(2) . .
C6 N4 C3 113.1(2) . .
C7 N4 C3 111.7(2) . .
N2 C1 N1 111.0(2) . .
N2 C1 H1A 109.4 . .
N1 C1 H1A 109.4 . .
N2 C1 H1B 109.4 . .
N1 C1 H1B 109.4 . .
H1A C1 H1B 108.0 . .
N2 C2 N4 110.0(2) . .
N2 C2 H2A 109.7 . .
N4 C2 H2A 109.7 . .
N2 C2 H2B 109.7 . .
N4 C2 H2B 109.7 . .
H2A C2 H2B 108.2 . .
O15 C3 N4 110.8(2) . .
O15 C3 H3A 109.5 . .
N4 C3 H3A 109.5 . .
O15 C3 H3B 109.5 . .
N4 C3 H3B 109.5 . .
H3A C3 H3B 108.1 . .
N2 C4 N3 110.9(2) . .
N2 C4 H4A 109.5 . .
N3 C4 H4A 109.5 . .
N2 C4 H4B 109.5 . .
N3 C4 H4B 109.5 . .
H4A C4 H4B 108.1 . .
N1 C5 N3 110.6(2) . .
N1 C5 H5A 109.5 . .
N3 C5 H5A 109.5 . .
N1 C5 H5B 109.5 . .
N3 C5 H5B 109.5 . .
H5A C5 H5B 108.1 . .
N1 C6 N4 109.59(19) . .
N1 C6 H6A 109.8 . .
N4 C6 H6A 109.8 . .
N1 C6 H6B 109.8 . .
N4 C6 H6B 109.8 . .
H6A C6 H6B 108.2 . .
N3 C7 N4 109.6(2) . .
N3 C7 H7A 109.7 . .
N4 C7 H7A 109.7 . .
N3 C7 H7B 109.7 . .
N4 C7 H7B 109.7 . .
H7A C7 H7B 108.2 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
V1 O11 1.6065(17) .
V1 O7 1.7544(17) .
V1 O6 1.8409(17) .
V1 O2 1.9911(17) .
V1 O4 2.1079(17) .
V1 O8 2.2819(15) .
V1 V4 3.0944(6) .
V1 V3 3.1142(6) .
V1 V2 3.1183(6) .
V2 O9 1.6749(17) .
V2 O3 1.6851(17) .
V2 O2 1.8839(16) .
V2 O4 2.0396(16) 2_666
V2 O8 2.0845(16) .
V2 O8 2.0866(15) 2_666
V2 V3 3.0726(6) .
V2 V4 3.0753(6) 2_666
V2 V5 3.1148(6) 2_666
V3 O13 1.5991(18) .
V3 O5 1.8194(18) .
V3 O1 1.8305(17) .
V3 O7 1.9388(17) .
V3 O3 2.0498(17) .
V3 O8 2.3272(16) .
V3 V4 3.0689(6) .
V3 V5 3.0816(6) .
V4 O14 1.6047(19) .
V4 O6 1.8183(17) .
V4 O5 1.8270(17) .
V4 O10 1.9392(17) .
V4 O9 2.0434(17) 2_666
V4 O8 2.3451(16) .
V4 V2 3.0753(6) 2_666
V5 O12 1.6008(18) .
V5 O10 1.7587(17) .
V5 O1 1.8410(17) .
V5 O2 1.9958(16) 2_666
V5 O2 1.9958(16) 2_666
V5 O4 2.0922(17) 2_666
V5 O8 2.2855(15) .
V5 V2 3.1148(6) 2_666
O1W H1WA 0.799(17) .
O1W H1WB 0.825(17) .
O2 V5 1.9958(16) 2_666
O2W H2WA 0.836(18) .
O2W H2WB 0.832(18) .
O3W H3WA 0.86(4) .
O3W H3WB 0.89(4) .
O4 V2 2.0396(16) 2_666
O4 V5 2.0922(17) 2_666
O4 H4 0.867(17) .
O8 V2 2.0866(15) 2_666
O9 V4 2.0434(17) 2_666
O12 H12 0.812(16) .
O15 C3 1.382(4) .
O15 H15 0.890(18) .
N1 C6 1.442(3) .
N1 C5 1.473(3) .
N1 C1 1.475(3) .
N2 C2 1.439(3) .
N2 C1 1.467(3) .
N2 C4 1.472(3) .
N3 C7 1.445(3) .
N3 C4 1.477(3) .
N3 C5 1.479(4) .
N4 C2 1.523(3) .
N4 C6 1.524(3) .
N4 C7 1.524(3) .
N4 C3 1.529(3) .
C1 H1A 0.9700 .
C1 H1B 0.9700 .
C2 H2A 0.9700 .
C2 H2B 0.9700 .
C3 H3A 0.9700 .
C3 H3B 0.9700 .
C4 H4A 0.9700 .
C4 H4B 0.9700 .
C5 H5A 0.9700 .
C5 H5B 0.9700 .
C6 H6A 0.9700 .
C6 H6B 0.9700 .
C7 H7A 0.9700 .
C7 H7B 0.9700 .
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
O1W H1WA N1 0.799(17) 2.12(2) 2.890(3) 162(3) 1_655
O1W H1WB O14 0.825(17) 2.080(18) 2.889(3) 167(3) 1_655
O2W H2WA O15 0.836(18) 2.29(3) 3.023(3) 147(4) 2_666
O2W H2WB N3 0.832(18) 2.29(3) 3.020(3) 147(4) 1_654
O3W H3WA O2W 0.86(4) 2.32(3) 3.125(5) 156(4) 2_656
O3W H3WB O2W 0.89(4) 2.08(2) 2.958(5) 171(5) 1_556
O4 H4 O1W 0.867(17) 1.797(18) 2.642(3) 164(3) 2_666
O15 H15 O14 0.890(18) 2.13(3) 2.866(3) 140(3) 2_566
C1 H1A O10 0.97 2.41 3.364(3) 168.5 2_556
C1 H1B O12 0.97 2.44 3.309(3) 149.0 .
C2 H2A O2 0.97 2.43 3.311(3) 150.2 2_666
C2 H2B O13 0.97 2.35 3.198(3) 146.0 1_556
C3 H3A O7 0.97 2.47 3.376(3) 156.1 1_556
C3 H3B O2 0.97 2.52 3.380(3) 147.3 2_666
C3 H3B O3 0.97 2.37 3.173(3) 139.2 2_666
C4 H4A O5 0.97 2.52 3.373(3) 146.8 1_556
C4 H4B O5 0.97 2.59 3.546(3) 169.6 2_556
C5 H5A O1 0.97 2.46 3.406(3) 163.5 2_556
C5 H5B O11 0.97 2.42 3.377(3) 170.3 2_566
C6 H6A O6 0.97 2.41 3.372(3) 174.3 2_566
C6 H6B O10 0.97 2.55 3.409(3) 147.8 .
C6 H6B O9 0.97 2.53 3.356(3) 142.9 2_666
C7 H7A O5 0.97 2.45 3.320(3) 149.5 1_556
C7 H7B O15 0.97 2.49 3.157(3) 126.1 2_567
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O11 V1 V2 O9 9.91(13) . .
O7 V1 V2 O9 109.50(10) . .
O6 V1 V2 O9 -160.28(11) . .
O2 V1 V2 O9 -4.07(11) . .
O4 V1 V2 O9 -81.66(10) . .
O8 V1 V2 O9 -159.62(11) . .
V4 V1 V2 O9 -166.70(9) . .
V3 V1 V2 O9 140.23(9) . .
O11 V1 V2 O3 -98.82(11) . .
O7 V1 V2 O3 0.76(8) . .
O6 V1 V2 O3 90.98(9) . .
O2 V1 V2 O3 -112.81(10) . .
O4 V1 V2 O3 169.60(7) . .
O8 V1 V2 O3 91.64(8) . .
V4 V1 V2 O3 84.56(6) . .
V3 V1 V2 O3 31.50(6) . .
O11 V1 V2 O2 13.99(12) . .
O7 V1 V2 O2 113.57(10) . .
O6 V1 V2 O2 -156.21(10) . .
O4 V1 V2 O2 -77.59(9) . .
O8 V1 V2 O2 -155.55(10) . .
V4 V1 V2 O2 -162.63(8) . .
V3 V1 V2 O2 144.31(8) . .
O11 V1 V2 O4 169.85(11) . 2_666
O7 V1 V2 O4 -90.56(8) . 2_666
O6 V1 V2 O4 -0.34(9) . 2_666
O2 V1 V2 O4 155.86(10) . 2_666
O4 V1 V2 O4 78.28(8) . 2_666
O8 V1 V2 O4 0.32(8) . 2_666
V4 V1 V2 O4 -6.76(6) . 2_666
V3 V1 V2 O4 -59.83(6) . 2_666
O11 V1 V2 O8 169.53(11) . .
O7 V1 V2 O8 -90.88(8) . .
O6 V1 V2 O8 -0.66(8) . .
O2 V1 V2 O8 155.55(10) . .
O4 V1 V2 O8 77.96(7) . .
V4 V1 V2 O8 -7.08(6) . .
V3 V1 V2 O8 -60.15(6) . .
O11 V1 V2 O8 94.67(11) . 2_666
O7 V1 V2 O8 -165.75(7) . 2_666
O6 V1 V2 O8 -75.53(8) . 2_666
O2 V1 V2 O8 80.68(9) . 2_666
O4 V1 V2 O8 3.09(6) . 2_666
O8 V1 V2 O8 -74.87(8) . 2_666
V4 V1 V2 O8 -81.95(4) . 2_666
V3 V1 V2 O8 -135.01(5) . 2_666
O11 V1 V2 V3 -130.32(10) . .
O7 V1 V2 V3 -30.74(6) . .
O6 V1 V2 V3 59.48(7) . .
O2 V1 V2 V3 -144.31(8) . .
O4 V1 V2 V3 138.10(5) . .
O8 V1 V2 V3 60.15(6) . .
V4 V1 V2 V3 53.067(14) . .
O11 V1 V2 V4 56.84(10) . 2_666
O7 V1 V2 V4 156.43(6) . 2_666
O6 V1 V2 V4 -113.35(7) . 2_666
O2 V1 V2 V4 42.85(8) . 2_666
O4 V1 V2 V4 -34.73(5) . 2_666
O8 V1 V2 V4 -112.69(6) . 2_666
V4 V1 V2 V4 -119.770(17) . 2_666
V3 V1 V2 V4 -172.84(2) . 2_666
O11 V1 V2 V5 53.56(10) . 2_666
O7 V1 V2 V5 153.15(6) . 2_666
O6 V1 V2 V5 -116.63(7) . 2_666
O2 V1 V2 V5 39.58(8) . 2_666
O4 V1 V2 V5 -38.01(5) . 2_666
O8 V1 V2 V5 -115.97(6) . 2_666
V4 V1 V2 V5 -123.048(15) . 2_666
V3 V1 V2 V5 -176.115(16) . 2_666
O9 V2 V3 O13 -10.66(14) . .
O3 V2 V3 O13 -2.95(12) . .
O2 V2 V3 O13 99.85(10) . .
O4 V2 V3 O13 -103.34(10) 2_666 .
O8 V2 V3 O13 177.68(11) . .
O8 V2 V3 O13 -177.50(10) 2_666 .
V5 V2 V3 O13 124.76(9) 2_666 .
V1 V2 V3 O13 120.72(9) . .
O9 V2 V3 O5 176.49(12) . .
O3 V2 V3 O5 -175.80(11) . .
O2 V2 V3 O5 -73.00(8) . .
O4 V2 V3 O5 83.81(8) 2_666 .
O8 V2 V3 O5 4.83(8) . .
O8 V2 V3 O5 9.65(9) 2_666 .
V5 V2 V3 O5 -48.09(7) 2_666 .
V1 V2 V3 O5 -52.13(7) . .
O9 V2 V3 O1 87.90(12) . .
O3 V2 V3 O1 95.61(10) . .
O2 V2 V3 O1 -161.59(7) . .
O4 V2 V3 O1 -4.78(7) 2_666 .
O8 V2 V3 O1 -83.75(8) . .
O8 V2 V3 O1 -78.94(8) 2_666 .
V5 V2 V3 O1 -136.68(6) 2_666 .
V1 V2 V3 O1 -140.71(6) . .
O9 V2 V3 O7 -103.72(11) . .
O3 V2 V3 O7 -96.02(10) . .
O2 V2 V3 O7 6.79(7) . .
O4 V2 V3 O7 163.59(7) 2_666 .
O8 V2 V3 O7 84.62(7) . .
O8 V2 V3 O7 89.43(7) 2_666 .
V5 V2 V3 O7 31.69(5) 2_666 .
V1 V2 V3 O7 27.66(5) . .
O9 V2 V3 O3 -7.71(13) . .
O2 V2 V3 O3 102.80(10) . .
O4 V2 V3 O3 -100.39(10) 2_666 .
O8 V2 V3 O3 -179.36(11) . .
O8 V2 V3 O3 -174.55(10) 2_666 .
V5 V2 V3 O3 127.71(9) 2_666 .
V1 V2 V3 O3 123.68(9) . .
O9 V2 V3 O8 171.66(12) . .
O3 V2 V3 O8 179.36(11) . .
O2 V2 V3 O8 -77.83(7) . .
O4 V2 V3 O8 78.97(7) 2_666 .
O8 V2 V3 O8 4.82(11) 2_666 .
V5 V2 V3 O8 -52.92(6) 2_666 .
V1 V2 V3 O8 -56.96(5) . .
O9 V2 V3 V4 174.88(10) . .
O3 V2 V3 V4 -177.42(9) . .
O2 V2 V3 V4 -74.61(5) . .
O4 V2 V3 V4 82.19(5) 2_666 .
O8 V2 V3 V4 3.22(5) . .
O8 V2 V3 V4 8.03(6) 2_666 .
V5 V2 V3 V4 -49.71(2) 2_666 .
V1 V2 V3 V4 -53.741(13) . .
O9 V2 V3 V5 117.97(10) . .
O3 V2 V3 V5 125.68(9) . .
O2 V2 V3 V5 -131.52(5) . .
O4 V2 V3 V5 25.29(5) 2_666 .
O8 V2 V3 V5 -53.69(5) . .
O8 V2 V3 V5 -48.87(5) 2_666 .
V5 V2 V3 V5 -106.613(18) 2_666 .
V1 V2 V3 V5 -110.646(15) . .
O9 V2 V3 V1 -131.38(10) . .
O3 V2 V3 V1 -123.68(9) . .
O2 V2 V3 V1 -20.87(5) . .
O4 V2 V3 V1 135.93(5) 2_666 .
O8 V2 V3 V1 56.96(5) . .
O8 V2 V3 V1 61.77(5) 2_666 .
V5 V2 V3 V1 4.033(17) 2_666 .
O11 V1 V3 O13 3.41(15) . .
O7 V1 V3 O13 -2.38(13) . .
O6 V1 V3 O13 107.35(11) . .
O2 V1 V3 O13 -100.25(11) . .
O4 V1 V3 O13 -170.32(11) . .
O8 V1 V3 O13 -171.07(11) . .
V4 V1 V3 O13 128.52(10) . .
V2 V1 V3 O13 -119.94(10) . .
O11 V1 V3 O5 -97.87(12) . .
O7 V1 V3 O5 -103.66(12) . .
O6 V1 V3 O5 6.08(7) . .
O2 V1 V3 O5 158.47(7) . .
O4 V1 V3 O5 88.40(8) . .
O8 V1 V3 O5 87.65(8) . .
V4 V1 V3 O5 27.24(5) . .
V2 V1 V3 O5 138.79(6) . .
O11 V1 V3 O1 174.35(13) . .
O7 V1 V3 O1 168.57(12) . .
O6 V1 V3 O1 -81.70(9) . .
O2 V1 V3 O1 70.70(8) . .
O4 V1 V3 O1 0.63(9) . .
O8 V1 V3 O1 -0.13(8) . .
V4 V1 V3 O1 -60.54(7) . .
V2 V1 V3 O1 51.01(7) . .
O11 V1 V3 O7 5.78(14) . .
O6 V1 V3 O7 109.73(12) . .
O2 V1 V3 O7 -97.87(11) . .
O4 V1 V3 O7 -167.94(12) . .
O8 V1 V3 O7 -168.69(12) . .
V4 V1 V3 O7 130.89(10) . .
V2 V1 V3 O7 -117.56(10) . .
O11 V1 V3 O3 97.58(12) . .
O7 V1 V3 O3 91.80(11) . .
O6 V1 V3 O3 -158.47(7) . .
O2 V1 V3 O3 -6.07(6) . .
O4 V1 V3 O3 -76.14(7) . .
O8 V1 V3 O3 -76.90(7) . .
V4 V1 V3 O3 -137.31(5) . .
V2 V1 V3 O3 -25.76(5) . .
O11 V1 V3 O8 174.48(12) . .
O7 V1 V3 O8 168.69(12) . .
O6 V1 V3 O8 -81.57(7) . .
O2 V1 V3 O8 70.82(7) . .
O4 V1 V3 O8 0.75(8) . .
V4 V1 V3 O8 -60.41(5) . .
V2 V1 V3 O8 51.14(5) . .
O11 V1 V3 V4 -125.11(11) . .
O7 V1 V3 V4 -130.89(10) . .
O6 V1 V3 V4 -21.16(5) . .
O2 V1 V3 V4 131.24(5) . .
O4 V1 V3 V4 61.16(6) . .
O8 V1 V3 V4 60.41(5) . .
V2 V1 V3 V4 111.548(16) . .
O11 V1 V3 V2 123.34(11) . .
O7 V1 V3 V2 117.56(10) . .
O6 V1 V3 V2 -132.71(5) . .
O2 V1 V3 V2 19.69(5) . .
O4 V1 V3 V2 -50.38(6) . .
O8 V1 V3 V2 -51.14(5) . .
V4 V1 V3 V2 -111.548(16) . .
O11 V1 V3 V5 -178.51(11) . .
O7 V1 V3 V5 175.70(10) . .
O6 V1 V3 V5 -74.57(5) . .
O2 V1 V3 V5 77.83(5) . .
O4 V1 V3 V5 7.76(6) . .
O8 V1 V3 V5 7.01(5) . .
V4 V1 V3 V5 -53.404(14) . .
V2 V1 V3 V5 58.144(14) . .
O13 V3 V4 O14 6.03(15) . .
O5 V3 V4 O14 2.29(14) . .
O1 V3 V4 O14 -98.87(12) . .
O7 V3 V4 O14 102.76(12) . .
O3 V3 V4 O14 178.26(12) . .
O8 V3 V4 O14 -177.28(12) . .
V2 V3 V4 O14 179.83(11) . .
V5 V3 V4 O14 -120.26(11) . .
V1 V3 V4 O14 125.72(11) . .
O13 V3 V4 O6 -98.31(12) . .
O5 V3 V4 O6 -102.05(12) . .
O1 V3 V4 O6 156.78(8) . .
O7 V3 V4 O6 -1.58(7) . .
O3 V3 V4 O6 73.91(8) . .
O8 V3 V4 O6 78.37(7) . .
V2 V3 V4 O6 75.49(6) . .
V5 V3 V4 O6 135.39(6) . .
V1 V3 V4 O6 21.38(6) . .
O13 V3 V4 O5 3.74(14) . .
O1 V3 V4 O5 -101.17(12) . .
O7 V3 V4 O5 100.47(11) . .
O3 V3 V4 O5 175.96(12) . .
O8 V3 V4 O5 -179.58(12) . .
V2 V3 V4 O5 177.54(10) . .
V5 V3 V4 O5 -122.56(10) . .
V1 V3 V4 O5 123.43(10) . .
O13 V3 V4 O10 103.98(11) . .
O5 V3 V4 O10 100.24(11) . .
O1 V3 V4 O10 -0.93(7) . .
O7 V3 V4 O10 -159.29(7) . .
O3 V3 V4 O10 -83.80(8) . .
O8 V3 V4 O10 -79.34(7) . .
V2 V3 V4 O10 -82.22(5) . .
V5 V3 V4 O10 -22.32(5) . .
V1 V3 V4 O10 -136.33(5) . .
O13 V3 V4 O9 178.39(11) . 2_666
O5 V3 V4 O9 174.65(12) . 2_666
O1 V3 V4 O9 73.49(8) . 2_666
O7 V3 V4 O9 -84.88(8) . 2_666
O3 V3 V4 O9 -9.38(8) . 2_666
O8 V3 V4 O9 -4.92(7) . 2_666
V2 V3 V4 O9 -7.80(6) . 2_666
V5 V3 V4 O9 52.10(6) . 2_666
V1 V3 V4 O9 -61.92(6) . 2_666
O13 V3 V4 O8 -176.68(11) . .
O5 V3 V4 O8 179.58(12) . .
O1 V3 V4 O8 78.41(7) . .
O7 V3 V4 O8 -79.96(7) . .
O3 V3 V4 O8 -4.46(7) . .
V2 V3 V4 O8 -2.88(5) . .
V5 V3 V4 O8 57.02(5) . .
V1 V3 V4 O8 -56.99(5) . .
O13 V3 V4 V2 -179.82(10) . 2_666
O5 V3 V4 V2 176.44(10) . 2_666
O1 V3 V4 V2 75.27(6) . 2_666
O7 V3 V4 V2 -83.09(5) . 2_666
O3 V3 V4 V2 -7.60(6) . 2_666
O8 V3 V4 V2 -3.14(5) . 2_666
V2 V3 V4 V2 -6.019(17) . 2_666
V5 V3 V4 V2 53.883(13) . 2_666
V1 V3 V4 V2 -60.130(14) . 2_666
O13 V3 V4 V1 -119.69(10) . .
O5 V3 V4 V1 -123.43(10) . .
O1 V3 V4 V1 135.40(6) . .
O7 V3 V4 V1 -22.96(5) . .
O3 V3 V4 V1 52.53(6) . .
O8 V3 V4 V1 56.99(5) . .
V2 V3 V4 V1 54.111(13) . .
V5 V3 V4 V1 114.013(16) . .
O11 V1 V4 O14 1.34(14) . .
O7 V1 V4 O14 -103.75(12) . .
O6 V1 V4 O14 8.19(14) . .
O2 V1 V4 O14 165.90(11) . .
O4 V1 V4 O14 99.19(11) . .
O8 V1 V4 O14 171.62(12) . .
V3 V1 V4 O14 -129.18(10) . .
V2 V1 V4 O14 177.89(10) . .
O11 V1 V4 O6 -6.85(14) . .
O7 V1 V4 O6 -111.95(12) . .
O2 V1 V4 O6 157.71(12) . .
O4 V1 V4 O6 91.00(11) . .
O8 V1 V4 O6 163.42(12) . .
V3 V1 V4 O6 -137.37(10) . .
V2 V1 V4 O6 169.70(10) . .
O11 V1 V4 O5 103.44(11) . .
O7 V1 V4 O5 -1.65(8) . .
O6 V1 V4 O5 110.30(12) . .
O2 V1 V4 O5 -91.99(8) . .
O4 V1 V4 O5 -158.71(7) . .
O8 V1 V4 O5 -86.28(8) . .
V3 V1 V4 O5 -27.08(6) . .
V2 V1 V4 O5 -80.01(6) . .
O11 V1 V4 O10 -174.42(11) . .
O7 V1 V4 O10 80.49(8) . .
O6 V1 V4 O10 -167.56(12) . .
O2 V1 V4 O10 -9.85(9) . .
O4 V1 V4 O10 -76.56(8) . .
O8 V1 V4 O10 -4.14(8) . .
V3 V1 V4 O10 55.07(6) . .
V2 V1 V4 O10 2.13(6) . .
O11 V1 V4 O9 -98.37(11) . 2_666
O7 V1 V4 O9 156.53(7) . 2_666
O6 V1 V4 O9 -91.52(11) . 2_666
O2 V1 V4 O9 66.19(7) . 2_666
O4 V1 V4 O9 -0.52(6) . 2_666
O8 V1 V4 O9 71.90(7) . 2_666
V3 V1 V4 O9 131.11(5) . 2_666
V2 V1 V4 O9 78.18(5) . 2_666
O11 V1 V4 O8 -170.28(11) . .
O7 V1 V4 O8 84.63(8) . .
O6 V1 V4 O8 -163.42(12) . .
O2 V1 V4 O8 -5.71(7) . .
O4 V1 V4 O8 -72.42(7) . .
V3 V1 V4 O8 59.21(5) . .
V2 V1 V4 O8 6.28(5) . .
O11 V1 V4 V3 130.52(10) . .
O7 V1 V4 V3 25.42(6) . .
O6 V1 V4 V3 137.37(10) . .
O2 V1 V4 V3 -64.92(6) . .
O4 V1 V4 V3 -131.63(5) . .
O8 V1 V4 V3 -59.21(5) . .
V2 V1 V4 V3 -52.932(14) . .
O11 V1 V4 V2 -122.60(10) . 2_666
O7 V1 V4 V2 132.31(6) . 2_666
O6 V1 V4 V2 -115.74(10) . 2_666
O2 V1 V4 V2 41.97(6) . 2_666
O4 V1 V4 V2 -24.75(4) . 2_666
O8 V1 V4 V2 47.68(5) . 2_666
V3 V1 V4 V2 106.885(15) . 2_666
V2 V1 V4 V2 53.952(15) . 2_666
O13 V3 V5 O12 0.45(15) . .
O5 V3 V5 O12 102.52(12) . .
O1 V3 V5 O12 -8.08(14) . .
O7 V3 V5 O12 -174.84(12) . .
O3 V3 V5 O12 -97.95(12) . .
O8 V3 V5 O12 -170.57(12) . .
V4 V3 V5 O12 129.99(11) . .
V2 V3 V5 O12 -122.76(11) . .
V1 V3 V5 O12 -177.51(11) . .
O13 V3 V5 O10 -104.92(12) . .
O5 V3 V5 O10 -2.85(8) . .
O1 V3 V5 O10 -113.45(12) . .
O7 V3 V5 O10 79.79(8) . .
O3 V3 V5 O10 156.68(7) . .
O8 V3 V5 O10 84.06(8) . .
V4 V3 V5 O10 24.62(6) . .
V2 V3 V5 O10 131.87(6) . .
V1 V3 V5 O10 77.12(6) . .
O13 V3 V5 O1 8.53(14) . .
O5 V3 V5 O1 110.59(12) . .
O7 V3 V5 O1 -166.76(12) . .
O3 V3 V5 O1 -89.87(11) . .
O8 V3 V5 O1 -162.49(12) . .
V4 V3 V5 O1 138.07(10) . .
V2 V3 V5 O1 -114.68(10) . .
V1 V3 V5 O1 -169.43(10) . .
O13 V3 V5 O2 165.89(12) . 2_666
O5 V3 V5 O2 -92.05(8) . 2_666
O1 V3 V5 O2 157.35(12) . 2_666
O7 V3 V5 O2 -9.41(9) . 2_666
O3 V3 V5 O2 67.48(7) . 2_666
O8 V3 V5 O2 -5.14(8) . 2_666
V4 V3 V5 O2 -64.58(6) . 2_666
V2 V3 V5 O2 42.68(6) . 2_666
V1 V3 V5 O2 -12.07(6) . 2_666
O13 V3 V5 O2 165.89(12) . 2_666
O5 V3 V5 O2 -92.05(8) . 2_666
O1 V3 V5 O2 157.35(12) . 2_666
O7 V3 V5 O2 -9.41(9) . 2_666
O3 V3 V5 O2 67.48(7) . 2_666
O8 V3 V5 O2 -5.14(8) . 2_666
V4 V3 V5 O2 -64.58(6) . 2_666
V2 V3 V5 O2 42.68(6) . 2_666
V1 V3 V5 O2 -12.07(6) . 2_666
O13 V3 V5 O4 98.57(11) . 2_666
O5 V3 V5 O4 -159.37(7) . 2_666
O1 V3 V5 O4 90.04(11) . 2_666
O7 V3 V5 O4 -76.72(8) . 2_666
O3 V3 V5 O4 0.17(6) . 2_666
O8 V3 V5 O4 -72.45(7) . 2_666
V4 V3 V5 O4 -131.90(5) . 2_666
V2 V3 V5 O4 -24.64(4) . 2_666
V1 V3 V5 O4 -79.39(5) . 2_666
O13 V3 V5 O8 171.02(12) . .
O5 V3 V5 O8 -86.91(8) . .
O1 V3 V5 O8 162.49(12) . .
O7 V3 V5 O8 -4.27(8) . .
O3 V3 V5 O8 72.62(7) . .
V4 V3 V5 O8 -59.44(5) . .
V2 V3 V5 O8 47.81(5) . .
V1 V3 V5 O8 -6.94(5) . .
O13 V3 V5 V2 177.59(10) . 2_666
O5 V3 V5 V2 -80.35(6) . 2_666
O1 V3 V5 V2 169.05(10) . 2_666
O7 V3 V5 V2 2.29(7) . 2_666
O3 V3 V5 V2 79.18(5) . 2_666
O8 V3 V5 V2 6.56(5) . 2_666
V4 V3 V5 V2 -52.881(14) . 2_666
V2 V3 V5 V2 54.375(15) . 2_666
V1 V3 V5 V2 -0.375(15) . 2_666
O13 V3 O1 V5 -173.83(10) . .
O5 V3 O1 V5 -68.06(10) . .
O7 V3 O1 V5 27.5(2) . .
O3 V3 O1 V5 87.21(10) . .
O8 V3 O1 V5 13.04(9) . .
V4 V3 O1 V5 -35.92(8) . .
V2 V3 O1 V5 56.32(8) . .
V1 V3 O1 V5 13.13(13) . .
O12 V5 O1 V3 174.26(10) . .
O10 V5 O1 V3 66.87(10) . .
O2 V5 O1 V3 -43.2(2) 2_666 .
O2 V5 O1 V3 -43.2(2) 2_666 .
O4 V5 O1 V3 -87.59(10) 2_666 .
O8 V5 O1 V3 -13.24(9) . .
V2 V5 O1 V3 -13.00(12) 2_666 .
O9 V2 O2 V1 177.20(8) . .
O3 V2 O2 V1 68.75(9) . .
O4 V2 O2 V1 -56.5(2) 2_666 .
O8 V2 O2 V1 -17.80(7) . .
O8 V2 O2 V1 -96.20(8) 2_666 .
V3 V2 O2 V1 30.51(6) . .
V4 V2 O2 V1 -144.93(6) 2_666 .
V5 V2 O2 V1 -113.88(10) 2_666 .
O9 V2 O2 V5 -68.92(9) . 2_666
O3 V2 O2 V5 -177.37(8) . 2_666
O4 V2 O2 V5 57.4(2) 2_666 2_666
O8 V2 O2 V5 96.09(8) . 2_666
O8 V2 O2 V5 17.68(7) 2_666 2_666
V3 V2 O2 V5 144.39(6) . 2_666
V4 V2 O2 V5 -31.04(7) 2_666 2_666
V1 V2 O2 V5 113.88(10) . 2_666
O11 V1 O2 V2 -169.88(9) . .
O7 V1 O2 V2 -64.14(9) . .
O6 V1 O2 V2 46.15(18) . .
O4 V1 O2 V2 93.57(8) . .
O8 V1 O2 V2 16.63(7) . .
V4 V1 O2 V2 21.08(10) . .
V3 V1 O2 V2 -30.04(6) . .
O11 V1 O2 V5 76.12(9) . 2_666
O7 V1 O2 V5 -178.14(7) . 2_666
O6 V1 O2 V5 -67.85(17) . 2_666
O4 V1 O2 V5 -20.43(7) . 2_666
O8 V1 O2 V5 -97.37(7) . 2_666
V4 V1 O2 V5 -92.92(7) . 2_666
V3 V1 O2 V5 -144.04(6) . 2_666
V2 V1 O2 V5 -114.00(10) . 2_666
O9 V2 O3 V3 175.37(8) . .
O2 V2 O3 V3 -81.36(9) . .
O4 V2 O3 V3 79.84(8) 2_666 .
O8 V2 O3 V3 0.48(8) . .
O8 V2 O3 V3 17.0(3) 2_666 .
V4 V2 O3 V3 169.92(3) 2_666 .
V5 V2 O3 V3 -83.75(10) 2_666 .
V1 V2 O3 V3 -46.56(7) . .
O13 V3 O3 V2 177.73(9) . .
O5 V3 O3 V2 8.3(2) . .
O1 V3 O3 V2 -80.77(9) . .
O7 V3 O3 V2 78.39(9) . .
O8 V3 O3 V2 -0.45(8) . .
V4 V3 O3 V2 3.07(11) . .
V5 V3 O3 V2 -47.62(7) . .
V1 V3 O3 V2 47.36(7) . .
O11 V1 O4 V2 171.60(9) . 2_666
O7 V1 O4 V2 -28.6(2) . 2_666
O6 V1 O4 V2 68.61(8) . 2_666
O2 V1 O4 V2 -90.89(8) . 2_666
O8 V1 O4 V2 -11.97(7) . 2_666
V4 V1 O4 V2 36.51(6) . 2_666
V3 V1 O4 V2 -12.55(9) . 2_666
V2 V1 O4 V2 -54.91(6) . 2_666
O11 V1 O4 V5 -78.66(9) . 2_666
O7 V1 O4 V5 81.17(18) . 2_666
O6 V1 O4 V5 178.35(7) . 2_666
O2 V1 O4 V5 18.86(6) . 2_666
O8 V1 O4 V5 97.78(7) . 2_666
V4 V1 O4 V5 146.26(5) . 2_666
V3 V1 O4 V5 97.19(6) . 2_666
V2 V1 O4 V5 54.84(5) . 2_666
O13 V3 O5 V4 -177.38(10) . .
O1 V3 O5 V4 79.12(10) . .
O7 V3 O5 V4 -76.90(10) . .
O3 V3 O5 V4 -8.2(2) . .
O8 V3 O5 V4 0.32(9) . .
V2 V3 O5 V4 -2.98(12) . .
V5 V3 O5 V4 48.36(8) . .
V1 V3 O5 V4 -47.12(8) . .
O14 V4 O5 V3 -178.39(10) . .
O6 V4 O5 V3 77.73(10) . .
O10 V4 O5 V3 -76.90(10) . .
O9 V4 O5 V3 -10.4(2) 2_666 .
O8 V4 O5 V3 -0.32(9) . .
V2 V4 O5 V3 -4.28(12) 2_666 .
V1 V4 O5 V3 47.43(8) . .
O14 V4 O6 V1 -174.05(10) . .
O5 V4 O6 V1 -68.16(10) . .
O10 V4 O6 V1 24.7(2) . .
O9 V4 O6 V1 85.89(10) 2_666 .
O8 V4 O6 V1 12.32(9) . .
V3 V4 O6 V1 -36.30(8) . .
V2 V4 O6 V1 55.58(8) 2_666 .
O11 V1 O6 V4 175.05(10) . .
O7 V1 O6 V4 68.12(10) . .
O2 V1 O6 V4 -41.5(2) . .
O4 V1 O6 V4 -86.62(10) . .
O8 V1 O6 V4 -12.61(9) . .
V3 V1 O6 V4 35.79(8) . .
V2 V1 O6 V4 -12.16(12) . .
O11 V1 O7 V3 -176.09(10) . .
O6 V1 O7 V3 -70.45(10) . .
O2 V1 O7 V3 82.94(10) . .
O4 V1 O7 V3 24.5(2) . .
O8 V1 O7 V3 8.47(9) . .
V4 V1 O7 V3 -40.78(8) . .
V2 V1 O7 V3 50.91(8) . .
O13 V3 O7 V1 178.18(10) . .
O5 V3 O7 V1 73.57(10) . .
O1 V3 O7 V1 -23.0(2) . .
O3 V3 O7 V1 -83.32(10) . .
O8 V3 O7 V1 -8.44(9) . .
V4 V3 O7 V1 41.41(8) . .
V2 V3 O7 V1 -52.25(8) . .
V5 V3 O7 V1 -5.21(12) . .
O9 V2 O8 V2 15.0(3) . 2_666
O3 V2 O8 V2 175.65(8) . 2_666
O2 V2 O8 V2 -84.22(7) . 2_666
O4 V2 O8 V2 81.27(7) 2_666 2_666
O8 V2 O8 V2 0.0 2_666 2_666
V3 V2 O8 V2 176.05(9) . 2_666
V4 V2 O8 V2 3.37(8) 2_666 2_666
V5 V2 O8 V2 -46.59(5) 2_666 2_666
V1 V2 O8 V2 -98.99(7) . 2_666
O9 V2 O8 V1 114.0(3) . .
O3 V2 O8 V1 -85.36(7) . .
O2 V2 O8 V1 14.77(6) . .
O4 V2 O8 V1 -179.74(7) 2_666 .
O8 V2 O8 V1 98.99(7) 2_666 .
V3 V2 O8 V1 -84.97(5) . .
V4 V2 O8 V1 102.36(5) 2_666 .
V5 V2 O8 V1 52.40(4) 2_666 .
O9 V2 O8 V5 -77.6(3) . .
O3 V2 O8 V5 83.10(7) . .
O2 V2 O8 V5 -176.77(7) . .
O4 V2 O8 V5 -11.28(6) 2_666 .
O8 V2 O8 V5 -92.55(7) 2_666 .
V3 V2 O8 V5 83.50(6) . .
V4 V2 O8 V5 -89.18(6) 2_666 .
V5 V2 O8 V5 -139.14(5) 2_666 .
V1 V2 O8 V5 168.46(8) . .
O9 V2 O8 V3 -161.1(3) . .
O3 V2 O8 V3 -0.40(7) . .
O2 V2 O8 V3 99.73(6) . .
O4 V2 O8 V3 -94.77(6) 2_666 .
O8 V2 O8 V3 -176.05(9) 2_666 .
V4 V2 O8 V3 -172.67(2) 2_666 .
V5 V2 O8 V3 137.36(4) 2_666 .
V1 V2 O8 V3 84.97(5) . .
O9 V2 O8 V4 175.5(4) . .
O3 V2 O8 V4 -23.8(4) . .
O2 V2 O8 V4 76.3(4) . .
O4 V2 O8 V4 -118.2(4) 2_666 .
O8 V2 O8 V4 160.6(5) 2_666 .
V3 V2 O8 V4 -23.4(4) . .
V4 V2 O8 V4 163.9(4) 2_666 .
V5 V2 O8 V4 114.0(4) 2_666 .
V1 V2 O8 V4 61.6(4) . .
O7 V1 O8 V2 81.59(7) . .
O6 V1 O8 V2 179.43(7) . .
O2 V1 O8 V2 -14.32(6) . .
O4 V1 O8 V2 -91.32(7) . .
V4 V1 O8 V2 170.59(8) . .
V3 V1 O8 V2 88.01(5) . .
O7 V1 O8 V2 -175.72(8) . 2_666
O6 V1 O8 V2 -77.88(7) . 2_666
O2 V1 O8 V2 88.37(7) . 2_666
O4 V1 O8 V2 11.37(6) . 2_666
V4 V1 O8 V2 -86.73(6) . 2_666
V3 V1 O8 V2 -169.30(9) . 2_666
V2 V1 O8 V2 102.69(8) . 2_666
O7 V1 O8 V5 -46.9(3) . .
O6 V1 O8 V5 51.0(3) . .
O2 V1 O8 V5 -142.8(3) . .
O4 V1 O8 V5 140.2(3) . .
V4 V1 O8 V5 42.1(3) . .
V3 V1 O8 V5 -40.5(3) . .
V2 V1 O8 V5 -128.5(3) . .
O7 V1 O8 V3 -6.42(7) . .
O6 V1 O8 V3 91.42(7) . .
O2 V1 O8 V3 -102.33(6) . .
O4 V1 O8 V3 -179.33(7) . .
V4 V1 O8 V3 82.58(5) . .
V2 V1 O8 V3 -88.01(5) . .
O7 V1 O8 V4 -89.00(7) . .
O6 V1 O8 V4 8.84(6) . .
O2 V1 O8 V4 175.10(6) . .
O4 V1 O8 V4 98.09(6) . .
V3 V1 O8 V4 -82.58(5) . .
V2 V1 O8 V4 -170.59(8) . .
O10 V5 O8 V2 -176.55(8) . .
O1 V5 O8 V2 -77.68(7) . .
O2 V5 O8 V2 88.39(7) 2_666 .
O2 V5 O8 V2 88.39(7) 2_666 .
O4 V5 O8 V2 11.25(6) 2_666 .
V3 V5 O8 V2 -87.20(6) . .
V2 V5 O8 V2 102.62(8) 2_666 .
O10 V5 O8 V2 80.83(7) . 2_666
O1 V5 O8 V2 179.70(7) . 2_666
O2 V5 O8 V2 -14.23(6) 2_666 2_666
O2 V5 O8 V2 -14.23(6) 2_666 2_666
O4 V5 O8 V2 -91.37(7) 2_666 2_666
V3 V5 O8 V2 170.18(8) . 2_666
O10 V5 O8 V1 -48.8(3) . .
O1 V5 O8 V1 50.1(3) . .
O2 V5 O8 V1 -143.9(3) 2_666 .
O2 V5 O8 V1 -143.9(3) 2_666 .
O4 V5 O8 V1 139.0(3) 2_666 .
V3 V5 O8 V1 40.5(3) . .
V2 V5 O8 V1 -129.6(3) 2_666 .
O10 V5 O8 V3 -89.35(7) . .
O1 V5 O8 V3 9.52(6) . .
O2 V5 O8 V3 175.60(7) 2_666 .
O2 V5 O8 V3 175.60(7) 2_666 .
O4 V5 O8 V3 98.45(6) 2_666 .
V2 V5 O8 V3 -170.18(8) 2_666 .
O10 V5 O8 V4 -6.78(6) . .
O1 V5 O8 V4 92.09(7) . .
O2 V5 O8 V4 -101.84(6) 2_666 .
O2 V5 O8 V4 -101.84(6) 2_666 .
O4 V5 O8 V4 -178.98(6) 2_666 .
V3 V5 O8 V4 82.57(5) . .
V2 V5 O8 V4 -87.61(5) 2_666 .
O5 V3 O8 V2 -175.98(7) . .
O1 V3 O8 V2 88.69(7) . .
O7 V3 O8 V2 -85.31(7) . .
O3 V3 O8 V2 0.34(6) . .
V4 V3 O8 V2 -175.75(7) . .
V5 V3 O8 V2 98.30(6) . .
V1 V3 O8 V2 -91.20(6) . .
O5 V3 O8 V2 24.3(4) . 2_666
O1 V3 O8 V2 -71.0(4) . 2_666
O7 V3 O8 V2 115.0(4) . 2_666
O3 V3 O8 V2 -159.4(4) . 2_666
V4 V3 O8 V2 24.5(4) . 2_666
V2 V3 O8 V2 -159.7(4) . 2_666
V5 V3 O8 V2 -61.4(4) . 2_666
V1 V3 O8 V2 109.1(4) . 2_666
O5 V3 O8 V1 -84.78(7) . .
O1 V3 O8 V1 179.90(7) . .
O7 V3 O8 V1 5.90(6) . .
O3 V3 O8 V1 91.54(6) . .
V4 V3 O8 V1 -84.55(5) . .
V2 V3 O8 V1 91.20(6) . .
V5 V3 O8 V1 -170.50(7) . .
O5 V3 O8 V5 85.72(7) . .
O1 V3 O8 V5 -9.60(6) . .
O7 V3 O8 V5 176.40(7) . .
O3 V3 O8 V5 -97.96(6) . .
V4 V3 O8 V5 85.95(5) . .
V2 V3 O8 V5 -98.30(6) . .
V1 V3 O8 V5 170.50(7) . .
O5 V3 O8 V4 -0.23(6) . .
O1 V3 O8 V4 -95.56(6) . .
O7 V3 O8 V4 90.45(6) . .
O3 V3 O8 V4 176.09(6) . .
V2 V3 O8 V4 175.75(7) . .
V5 V3 O8 V4 -85.95(5) . .
V1 V3 O8 V4 84.55(5) . .
O6 V4 O8 V2 -71.2(4) . .
O5 V4 O8 V2 23.8(4) . .
O10 V4 O8 V2 114.3(4) . .
O9 V4 O8 V2 -160.8(4) 2_666 .
V3 V4 O8 V2 23.6(4) . .
V2 V4 O8 V2 -161.0(5) 2_666 .
V1 V4 O8 V2 -62.2(4) . .
O6 V4 O8 V2 89.86(7) . 2_666
O5 V4 O8 V2 -175.14(7) . 2_666
O10 V4 O8 V2 -84.69(7) . 2_666
O9 V4 O8 V2 0.26(6) 2_666 2_666
V3 V4 O8 V2 -175.37(7) . 2_666
V1 V4 O8 V2 98.86(6) . 2_666
O6 V4 O8 V1 -8.99(6) . .
O5 V4 O8 V1 86.00(7) . .
O10 V4 O8 V1 176.45(7) . .
O9 V4 O8 V1 -98.60(6) 2_666 .
V3 V4 O8 V1 85.77(5) . .
V2 V4 O8 V1 -98.86(6) 2_666 .
O6 V4 O8 V5 -179.19(7) . .
O5 V4 O8 V5 -84.19(7) . .
O10 V4 O8 V5 6.25(6) . .
O9 V4 O8 V5 91.20(6) 2_666 .
V3 V4 O8 V5 -84.42(5) . .
V2 V4 O8 V5 90.95(5) 2_666 .
V1 V4 O8 V5 -170.20(7) . .
O6 V4 O8 V3 -94.76(6) . .
O5 V4 O8 V3 0.23(6) . .
O10 V4 O8 V3 90.68(6) . .
O9 V4 O8 V3 175.63(6) 2_666 .
V2 V4 O8 V3 175.37(7) 2_666 .
V1 V4 O8 V3 -85.77(5) . .
O3 V2 O9 V4 -174.86(8) . 2_666
O2 V2 O9 V4 81.91(9) . 2_666
O4 V2 O9 V4 -79.54(9) 2_666 2_666
O8 V2 O9 V4 -15.0(3) . 2_666
O8 V2 O9 V4 -0.37(8) 2_666 2_666
V3 V2 O9 V4 -169.85(3) . 2_666
V5 V2 O9 V4 46.85(7) 2_666 2_666
V1 V2 O9 V4 84.43(10) . 2_666
O12 V5 O10 V4 -176.24(10) . .
O1 V5 O10 V4 -70.02(10) . .
O2 V5 O10 V4 83.92(10) 2_666 .
O2 V5 O10 V4 83.92(10) 2_666 .
O4 V5 O10 V4 26.6(2) 2_666 .
O8 V5 O10 V4 9.09(9) . .
V3 V5 O10 V4 -39.93(8) . .
V2 V5 O10 V4 51.71(8) 2_666 .
O14 V4 O10 V5 177.18(10) . .
O6 V4 O10 V5 -21.5(2) . .
O5 V4 O10 V5 72.42(10) . .
O9 V4 O10 V5 -83.68(10) 2_666 .
O8 V4 O10 V5 -9.01(9) . .
V3 V4 O10 V5 40.38(8) . .
V2 V4 O10 V5 -52.97(8) 2_666 .
V1 V4 O10 V5 -5.89(12) . .
C2 N2 C1 N1 -60.2(3) . .
C4 N2 C1 N1 59.5(3) . .
C6 N1 C1 N2 60.4(3) . .
C5 N1 C1 N2 -59.7(3) . .
C1 N2 C2 N4 59.6(2) . .
C4 N2 C2 N4 -59.7(3) . .
C6 N4 C2 N2 -58.7(2) . .
C7 N4 C2 N2 58.5(3) . .
C3 N4 C2 N2 179.1(2) . .
C2 N4 C3 O15 178.3(2) . .
C6 N4 C3 O15 59.5(3) . .
C7 N4 C3 O15 -63.2(3) . .
C2 N2 C4 N3 60.8(3) . .
C1 N2 C4 N3 -59.0(3) . .
C7 N3 C4 N2 -60.9(3) . .
C5 N3 C4 N2 58.8(3) . .
C6 N1 C5 N3 -60.8(3) . .
C1 N1 C5 N3 59.2(3) . .
C7 N3 C5 N1 60.7(3) . .
C4 N3 C5 N1 -59.0(3) . .
C5 N1 C6 N4 59.6(3) . .
C1 N1 C6 N4 -59.7(3) . .
C2 N4 C6 N1 58.7(3) . .
C7 N4 C6 N1 -58.4(3) . .
C3 N4 C6 N1 177.2(2) . .
C4 N3 C7 N4 59.6(3) . .
C5 N3 C7 N4 -59.7(3) . .
C2 N4 C7 N3 -58.3(3) . .
C6 N4 C7 N3 58.5(3) . .
C3 N4 C7 N3 -176.2(2) . .
